Investigation of the effective parameters on welding residual stress in GTAW of
aluminum cylindrical shell
Yousef Ghaderi Dehkordia, Ali Pourkamali Anarakia* & Amir Reza Shahanib
Department of Mechanical Engineering, Shahid Rajaee Teacher Training University, Tehran 16758 136, Iran b
Faculty of Mechanical Engineering , K.N. Toosi University of Technology, Tehran 16765 3381, Iran
Received:27 August 2018; Accepted:22 August 2019
The present work aims to study the influence of different geometrical, technological, and material parameters on residual stress in tungsten inert gas butt-welded aluminum cylinder. In order to present a simple analytical model to estimate the welding residual stress, the Taguchi L18 array has been employed with one 6-level factor and four 3-level factors. A 3D coupled thermo-mechanical finite element model considering temperature-dependent material properties has been developed to determine the welding residual stress in all experiments. The numerical model has been validated using the hole-drilling method. Using statistical analysis, the order of factors based on their effect on residual stress has been determined as yield strength, length, thickness, heat input, and finally diameter. The residual stress increases with an increase in yield strength, diameter, and heat input, while decreases with an increase in thickness. Contribution of each parameter on residual stress has been specified using variance analysis; yield strength with 99.6% contribution is the most significant factor, while diameter has insignificant impact. Finally, high accuracy equations have been proposed to calculate the welding residual stress. Keywords: Welding residual stress, Finite element, Experimental design, Taguchi, Aluminum, Cylindrical shell 1 Introduction
Welding technology is widely used in production, maintenance and repair of structures. However, the high-localized heating and subsequent cooling lead to generation of tensile residual stress near to the weld line, which has adverse effect on performance of the welded components1-3. Therefore, an accurate evaluation of the welding residual stress is essential to assess the safety and tolerability of structures. During the past years, numerical methods based on the finite element (FE) analysis have been developed to simulate the welding process. For example, the FE technique was used to study the residual stress and distortion fields in welded aluminum stiffened plates 4, butt-welded Monel plates5, combined butt and fillet weld joint of steel plates6, welded steel stiffened plates7, and welded pipe joint of dissimilar steels8. Xu
studied the effect of metal strength on the residual stress in steel welded joins based on the experimental measurement and FE simulation. Pandey et al.10 developed a 3D FE analysis to study the effect of welding direction on residual deformation and temperature history in the submerged arc welding of double-sided fillet joints. They
conducted the experimental measurements to verify the numerical results successfully. Pandey et al.11 also used the FE method to study the effect of diffusible hydrogen in deposited metal in multipass welded steels. Chaurasia et al.12 studied the residual stresses of different welding methods experimentally. They measured the residual stresses of friction stir welding and tungsten inert gas (TIG) welding in welded steel plates using the hole-drilling method. It was observed that the magnitude of longitudinal residual stress of TIG welded joints was higher than friction stir welded joint. Javadi et al.13 investigated the clamping effect on welding residual stress of stainless steel plates by using the ultrasonic stress measurement method and FE analysis. They concluded that using the clamp significantly influences the deformation and the residual stress fields in the base metal. Ye et al.14 studied the influences of weld groove type on residual stress in a butt-welded joint by means of numerical simulation and experiment. It was concluded that the groove shape has a significant influence on welding residual stress. Pandey et al.15 evaluated the effect of grove design and number of welding pass on the transverse residual stress in the TIG welding of P91 steel pipes. They showed that the shrinkage stress in the narrow groove is less than that of the conventional ——————
V-groove. Similar results were reported by Giri et al.16. Pandey et al.17 reviewed the microstructure evolution and the mechanical properties of welded P91 steel pipes in different heat treatment condition. It was demonstrated that to obtain the desired properties and microstructure, it is necessary to perform the proper heat treatment after welding18-20. They also reported that re-austenitizing based tempering produced uniform microstructure and hardness across the weld joints in the TIG welding of dissimilar P91 and P92 steels21. The thermo-mechanical elastic plastic FE method cannot be used to calculate welding deformation of large and complex welded structures due to the limitation of computing speed. Hence, Vishvesha et al.22 used the elastic FE method based on the inherent strain theory to predict distortion in a welded ring of the guide blade carrier of a steam turbine. Several studies have been conducted to investigate the effects of process variables such as the heat input parameters23, 24 and welding sequence25 on welding residual stress of steel alloys.
According to the literature, it is clear that despite the vast research on welding simulation, there has been no analytical model to predict the influence of effective parameters on welding residual stress, especially for welded cylindrical shells of the work-hardened aluminum of 5000-Series. Further, experimental design is a beneficial method to identify the effective parameters and their impacts on the response variable. In this paper, experimental design is conducted to study the influence of various effective parameters on residual stress in axially welded aluminum cylinders. It is worth pointing out the axial weld in thin cylindrical vessels is a critical joint where the damage often initiated. Here, thickness, diameter, and length of the cylinder were selected as the geometrical parameter, heat input was selected as the technological parameters, and the yield strength of the base material was chosen as the material parameter. In order to provide a new simple analytical model, the Taguchi L18 array is employed with one 6-level factor and four 3-level factors. First, a 3D thermo elasto-plastic FE model, considering temperature-dependent material properties and a
moving volumetric heat source, is developed to determine the welding residual stress in experiments, by the ABAQUS software. The FE model is successfully validated by the experimental measurement of stresses. Using statistical analysis, the order of factors based on their effect on welding residual stress is determined as the yield strength, length, thickness, heat input, and finally diameter. In addition, the residual stress increases with an increase in the yield strength, diameter, and heat input, while decreases with an increase in the thickness. Further, contribution of each parameter on the welding residual stress is determined using variance analysis. Finally, high accuracy equations are proposed that can be used to calculate the welding residual stress in terms of design factors.
2 Experimental Procedure
In order to verify the FE analysis, the residual stresses on the outside surface of the axially welded cylinder were measured using the experimental method.
2.1 Material and specimen preparation
The experimental specimen was prepared through axial welding of a cylindrical shell with diameter 800 mm, length 500 mm, and thickness 2 mm. The material is a non-heat-treatable aluminum of 5000-Series that is strengthened through cold-working process. The alloy has excellent corrosion resistance, moderately high strength, and good welding qualities without the necessity for post-weld treatment26. This alloy commonly used in the manufacture of high strength welded structures, pressure vessels, marine components, and storage tanks. The optical emission spectroscopy was utilized to determine the chemical composition of the alloy and the results are given in Table 1. The thermo-physical properties of the material are shown in Fig. 127.
The welding process is the gas tungsten arc welding (GTAW) that used the non-consumable electrode made of pure tungsten and the high purity (99.99%) argon as shielding gas. The single-pass welding was done by automatic welding machine with the process Table 1 — Chemical composition of the investigated aluminum.
Element Al Mg Ti Zn Mn Cu Fe Si
% 92.52 6.36 0.048 0.074 0.648 0.026 0.181 0.161
Element Cr Sb Be Zr B Sn Pb Ni
parameters given in Table 2. These values were selected according to a prequalified welding procedure specifications, in which the range of current is 140-180 A, range of gas flow rate is 10-15 L/Min, and the power supply will maintain the user selected current by automatically adjusting the voltage supplied (constant current mode). During welding, the specimens were restricted at the top with two clamps at a distance of 16 mm from the weld centerline. Due to the high effect of yield strength on welding residual stress, the mechanical specifications of the material were obtained in elevated temperatures by high-temperature tensile test, based on the ASTM E 21 standard28, as shown in Fig. 2. The specimen geometry and the prepared specimens, which were exploited for this test, are shown in Fig. 3.
2.2 Residual stress measurement
Over the years, several methods have been developed to measure the welding residual stress in different types of components29. The hole-drilling method is the most widely used technique for measuring the residual stresses. It offers advantages of good accuracy and reliability, standardized test
procedure, non-significant damage, and convenient practical implementation30. In this study, this method was utilized to measure the welding residual stresses. For strain measurement, five strain gauges of type delta rosette were attached to the top surface of the specimen after welding as shown in Fig.4.
3 Welding Simulation of Axial Butt Weld in the Cylindrical Shell
3.1 General considerations
A 3D FE model was developed in ABAQUS software, using the element birth technique based on
Fig. 1 — Thermal properties of the materials versus temperature. Table 2 — Parameters of the welding procedure. Current-AC (A) Voltage (V) Speed (cm/Min) Shielded gas
Gas flow rate (L/Min)
170 10 9.6 Argon 12
Fig. 2 — Mechanical properties of the materials versus temperature.
Fig. 3 — (a) Specimen geometry and (b) prepared specimen used for high temperature tensile test.
Fig. 4 — Welding residual stress measurement (a) gauge positions and (b) hole drilling machine.
the thermo-mechanical couple method. In this method, the temperature history was determined by the thermal analysis, and the subsequent mechanical analysis was performed by applying the predicted temperatures as the initial load. The analysis is composed of three stages as presented in Table 3. In the thermal analysis, the heat transfer element DC3D20 was employed, and in the mechanical analysis, the reduced integration element C3D20R was used. The thermal gradient is larger at the welding zone, so the finer mesh size was applied near the weld line as shown in Fig. 5. In order to reduce computation time, half symmetry condition was applied in the FE model. For the boundary condition, the restrictions due to the clamps of welding machine should be considered. Therefore, the nodes of the elements at distance 16 mm away from the weld centerline were clamped during welding process, and then released due to removing the clamps. The effect of mesh size, was investigated for four FE models as shown in Fig. 6. Based on the method proposed by Malik et al.31, the peak temperature was selected as the investigated parameter in the mesh sensitivity analysis. It is clear that the temperature is independent of the mesh size beyond 16000 elements.
Therefore, the model No. 3 was selected for the further analysis.
3.2. Thermal analysis
The Goldak's model32 was used for the heat source modelling as illustrated schematically in Fig. 7. In this model, the heat flux distribution for the front and the
Table 3 — Stages of the FE analysis. Stage number Stage time (s) Stage specification
Stage 1 312.5 Heating (welding time)
Stage 2 2500 Cooling
Stage 3 1 Releasing the clamps
Fig. 5 — FE model for the welding simulation.
Fig. 6 — Mesh sensitivity analysis in different models.
rear ellipsoids were presented respectively, as follows: 𝑞 𝑥, 𝑦, 𝑧 √ √ 𝑒𝑥𝑝 … (1) 𝑞 𝑥, 𝑦, 𝑧 √ √ 𝑒𝑥𝑝 … (2)
where, af, ar, 𝑏, and 𝑐 are the dimensional constants of
the Goldak's model, parameter 𝑄 is the total heat power, and parameter η is the thermal efficiency which is assumed to be 70% for the TIG welding33. The parameters ff and fr are the heat fraction
coefficients in the front and the rear ellipsoids, respectively, where ff + fr =232. Here, af, ar, b, and
c are considered 4, 12, 4, and 2 mm, respectively and ff and fr are 1.5 and 0.5.
In the thermal analysis, to calculate the heat flux within the elements, a user subroutine, namely, DFLUX, is developed. Another subroutine, called FILM, is developed to account for the heat loss coefficient. For simplicity, this coefficient is defined as a combination of convection and radiation coefficients as follow25:
ℎ ℎ 𝜀𝜎 𝑇 𝑇 𝑇 𝑇
where, ℎ is the convection heat transfer coefficient (8 W/m ℃), 𝜀 denotes emissivity (0.2), 𝜎 is the Stefan-Boltzman constant (5.67 10 W/m K ) 25, and 𝑇
is the ambient temperature.
3.3. Mechanical analysis
Total strain rate during welding is decomposed as follow25:
𝜀 𝜀 𝜀 𝜀 𝜀 … (4)
where, 𝜀 , 𝜀 , 𝜀 , and 𝜀 denote the strain rate components due to elastic, plastic, thermal loading, and phase transformation, respectively. During welding of the 5000-Series aluminum, phase transformation does not occur, so 𝜀 component is not considered.
3.4. Results and analysis of welding simulation
Fig. 8 shows the predicted temperature history during the welding. The monitoring points 1 and 2 have zero and 8 mm distance from the weld
centerline, respectively. It is expected that the monitoring point 1 exhibits the higher temperature compared to the monitoring point 2. As seen, at the time that the heat source intersects the line of monitoring points, the highest temperatures are achieved. The welding temperature histories are specified by a rapid heating, high peak temperature, rapid cooling, and returning to ambient temperature.
Fig. 9 shows the comparison of the axial and the hoop residual stresses of the FE method and the experimental measurement. As seen, the maximum axial residual stress (300 MPa) equals to the yield strength of the shell material approximately. Whereas, the global maximum value of the hoop residual stress
Fig. 8 — Welding temperature history at monitoring points.
(65 MPa) is much lower than the yield strength. Hence, a good agreement is observed between the FE analysis and the experimental method.
4 Design of Experiments
Since there are many effective factors on the welding analysis, design of experiments using the Taguchi technique34 was employed to evaluate the effect of main factors on the welding residual stress.
The Taguchi method is an important tool for design of experiments that offers a simple, efficient and systematic approach to optimize designs for performance, quality, and cost. This technique causes a decrease in the number of experiments with no reduction of accuracy from the full factorial method. Its simplicity in data collection, as well as practicality in designing the process parameters, makes design of experiment possible in any product and process optimization. Hence, it is strongly recommended to use this technique in improving the process quality. In the Taguchi approach, the design of experiment process will consider all the main factors and their influence on the response variable. This method presents guidance on which factors are significant to be controlled and which levels are suitable to put quality characteristic on target.35,36
Here, thickness (t), diameter (d), and length of the cylinder (l) were selected as the geometrical parameters, heat input (q) was selected as the technological parameter, and the yield strength of the base material (Sy) was chosen as the material
parameter. All parameters were studied in three levels, except the thickness, which was investigated in six levels. According to the number of design factors and their levels, the Taguchi's L18 orthogonal array was used in this study to conduct the experiments. The investigated factors and their levels are shown in Table 4. The maximum value of the axial welding residual stress was selected as the response variable.
Using the FE analysis, the response variables were determined for all experiments, as compared in Fig. 10. (I) Taguchi analysis: Taguchi analysis was performed and the results are given in Table 5. This table presents the maximum axial residual stress for every level of design parameters. In this table, the Delta parameter is the maximum difference of response variable between the levels of each factor, and the
Table 4 — The design factors and their levels. Exp. no. t (mm) d (mm) L (mm) q (W) Sy (MPa)
1 1 800 500 500 170 2 1 1600 1000 600 240 3 1 2400 1500 700 310 4 2 800 500 600 240 5 2 1600 1000 700 310 6 2 2400 1500 500 170 7 3 800 1000 500 310 8 3 1600 1500 600 170 9 3 2400 500 700 240 10 4 800 1500 700 240 11 4 1600 500 500 310 12 4 2400 1000 600 170 13 5 800 1000 700 170 14 5 1600 1500 500 240 15 5 2400 500 600 310 16 6 800 1500 600 310 17 6 1600 500 700 170 18 6 2400 1000 500 240
Table 5 — Average values of the maximum axial residual stress in every level of each factor (MPa).
Level t d l q Sy 1 236.3 234.7 235.7 234.0 166.8 2 235.3 235.3 232.8 236.8 235.0 3 235.3 235.3 236.8 234.5 303.5 4 233.0 - - - - 5 236.7 - - - - 6 234.0 - - - - Delta 3.7 0.7 4.0 2.8 136.7 Rank 3 5 2 4 1
Rank parameter specifies the rank of each factor based on the Delta values. As seen, the yield strength and the shell diameter are the two parameters with the most and the least effects, respectively.
This can be also observed in the plot of design factor impacts shown in Fig. 11. As seen, the yield strength affects the response variable significantly; an increase in the yield strength causes the welding residual stress to increase, while the effect of the shell diameter is rather insignificant. As determined from the rank values, the order of factors based on their effect on the axial residual stress is as follows: yield strength, length, thickness, heat input, and finally diameter.
(II) Regression analysis: The regression analysis was performed to derive the relationship between the design factors and the response variable. By this method, the maximum value of axial welding residual stress was estimated through the first order regression by Eqs. (5) and (6), as follows:
𝜎 2.48 0.286𝑡 0.00042𝑑 0.00117𝑙
0.0025𝑞 0.9556 … (5)
𝜎 97.11 0.286𝑡 0.33𝑑 0.58𝑙 0.25𝑞
68.33𝑆 … (6)
The above equations actually represent a single relationship with the same result. Eq. (5) is the numerical and Eq. (6) is the encoded forms of the relationship. For instance, for a yield strength of 240 MPa, one should place 240 as 𝑆 in Eq. (5); however, it has to be replaced by 2 in Eq. (6) according to Table 4. The numerical form is proposed for simplicity of calculations, which does not require dividing of the parameters and encoding.
Similar to the first order equations, second order equations were presented in the numerical and the encoded forms; Eq. (7) is the numerical and Eq. (8) is the encoded forms, as follows:
𝜎 90 1.08𝑡 0.00042𝑑 0.026𝑙 0.312𝑞 1.075𝑆 0.113𝑡 0.000014𝑙 0.00026𝑞 0.00025𝑆 … (7) 𝜎 101.5 1.08𝑡 0.333𝑑 13.082𝑙 10.58𝑞 67.67𝑆 0.113𝑡 3.42𝑙 2.58𝑞 0.17𝑆 … (8)
In the regression analysis, 𝑅 is the percentage of variation in the response explained by the model. In this study, the values of 𝑅 (𝑅 %99) indicate that the fit of the experimental data to the model is satisfactory.
(III) Analysis of Variance: The Analysis of Variance (ANOVA) was performed to understand how much change of each variable has contributed, as well as which variable is statistically important. The ANOVA results for the second order regression are shown in Table 6. The sum of squares indicates the relative importance of each factor; the factor with the biggest sum of squares has the greatest impact. The p-value also shows the significance level of each factor; a smaller p-value corresponds to a greater significance. Table 6 indicates that the yield strength (p=0.00), length (p=0.08), thickness (p=0.14), heat input (p=0.63), and diameter (p=0.73) in this order are the most significant factors affecting axial residual stress.
Fig. 11 — Effect of design factors on the axial residual stress.
Table 6 — ANOVA results for the axial residual stress. Source Sum of squares p-Value Contribution
t 27.1 0.14 0.03% d 1.3 0.73 0.00% l 41.9 0.08 0.04% q 2.5 0.63 0.01% Sy 513.0 0.00 99.61% t*t 1.4 0.72 0.00% l*l 46.7 0.07 0.08% q*q 26.7 0.15 0.05% Sy*Sy 6.4 0.45 0.03%
In addition, the yield strength with 99.6% contribution has the most impact on the axial residual stress. Note that these conclusions are completely compatible with the Taguchi results.
Figures 12 and 13 show the residual plot for the proposed first and second order equations, respectively. This plot is helpful in assessing whether the model satisfies the assumptions of the analysis. The residuals assumed to be random and normally
disturbed. Histogram of the residuals indicates that the data is normally disturbed. In addition, the residual versus order plots displays no pattern in data distribution. This proves that the residuals are independent from one another. As seen, the maximum residual value of the second order equation is 4.5, which is acceptably improved compared with the first order equation in which maximum residual value is 6.5.
Fig. 12 — Residual plots for the first order equation.
In order to verify the regression analysis, the results of the FE analysis were compared with the equation values as presented in Table 7. As seen, the relative difference of Eqs (5) and (7) are less than 3.37% and 2.59%, respectively, which are related to Experiment 12. This is compatible with the residual plots shown in Figs. 11 and 12.
This paper studied the influence of the main effective factors on the welding residual stress in the thin-walled cylinder of work-hardened Aluminum alloy. First, the 3D FE analysis of axial welding of the cylindrical shell was developed for predicting the welding residual stress. To validate the FE simulation, the residual stresses were measured through the hole drilling method. Next, the Taguchi experimental design method was applied to investigate the effect of various geometrical, technological and the material variables on the welding residual stress. In summary, the following conclusions can be drawn:
(1) The developed FE analysis gives accurate results for welding residual stress, so it can be used to obtain the values of response variable in the experimental design. (2) The yield strength, the cylinder length, the cylinder thickness, the heat input, and the cylinder diameter in this order are the most significant design factors affecting the axial welding residual stress.
(3) The yield strength is recognized as the most important parameter, while the diameter has insignificant impact on the axial residual stress.
(4) The welding residual stress increases with an increase in the yield strength, the diameter, and the heat input and decreases with an increase in the thickness. (5) The closed form equations are proposed to calculate the axial welding residual stress based on the thickness, diameter, length, heat input, and yield strength, with high accuracy
1 Xiu J, Li Y & Cheng Y, J Adhes Sci Technol, 32 (2017) 1. 2 Cui C, Zhang Q, Bao Y, Kang J & Bu Y, J Constr Steel Res,
148 (2018) 450.
3 Zhang W, Jiang W, Zhao X & Tu S T, Int J Fatigue, 109 (2018) 182.
4 Farajkhah V & Liu Y, Mar Struct, 50 (2016) 95. 5 Javadi Y, J Press Vessel Technol, 137 (2015) 011.
6 Kumanan S & Vaghela S, Ind J Eng Mater S, 24 (2017) 201. 7 Chen B Q & Soares C G, Int J Adv Technol, 86 (2016) 2723. 8 Xia J & Jin H, Int J Precis Eng Man, 19 (2018) 57.
9 Xu M, Chen J, Jin Y, Li Y & Lu H, Sci Technol Weld Joi, 20 (2015) 208.
10 Pandey C, Giri A & Mahapatra M M , Int J Steel Struct, 16 (2016) 333.
11 Pandey C, Mahapatra M M, Kumar P & Saini N, Metall and
Mater Trans B, 49 ( 2018) 2881.
12 Chaurasia P K, Pandey C, Giri A, Saini N & Mahapatra M M,
Arch Metall Mater, 63 (2017) 1019.
13 Javadi Y, Hasani M & Sadeghi S, J Non destruct Eval, 34 (2015) 3.
14 Ye Y, Cai J, Jiang X, Dai D & Deng D, Adv Eng Softw 86 (2015) 39.
15 Pandey C, Narang H K, Saini N, Mahapatra M M & Kumar P, Int J Steel Struct, 17 (2017) 763.
16 Giri A, Mahapatra M M, Sharma K & Singh P K,
Int J Steel Struct 17 (2017) 65.
17 Pandey C, Mahapatra M M, Kumar P & Saini N,
J Alloy Compd, 743 (2018) 332.
18 Pandey C & Mahapatra M M, J Mater Eng Perform, 25 (2016) 2195.
19 Pandey C, Mahapatra M M, Kumar P & Kumar S,
J Mater Process Technol, 266 (2019) 140.
20 Pandey C, Mahapatra M M, Kumar P & Giri A,
Met Mater Int, 23 (2017) 900.
21 Pandey C, Mahapatra M M, Kumar P & Saini N,
J Press Vessel Technol, 140 (2018) 214071.
22 Vishvesha A, Pandey C, Mahapatra M M & Mulik R S,
Int J Steel Struct, 17 (2017) 53.
23 Kamble A G & Rao R V, Indian J Eng Mater S, 24 (2017) 413.
24 Shokri V, Sadeghi S, Sadeghi M H & Javadi Y,
J Non destruct Eval, 34 (2015) 27.
25 Fu G, Lourenço M I, Duan M & Estefen S F, Marine Struct, 46 (2016) 30.
26 Fonda R W, Pao P S, Jones H N, Feng C R, Connolly B J & Davenport A J, Mater Sci Eng A, 519 (2009) 1.
Table 7 — Comparison between the results of FEM and equations (MPa).
Exp. no. FEM First order equation Second order equation Eq. (5) Difference (%) Eq. (7) Difference (%) 1 168 166.8 -0.70 166.8 -0.68 2 238 234.9 -1.31 235.5 -1.03 3 303 305.8 0.93 306.4 1.12 4 234 233.7 -0.14 237.1 1.31 5 302 304.6 0.86 300.9 -0.36 6 170 168.4 -0.96 168.6 -0.83 7 298 303.5 1.84 299.6 0.53 8 171 168.0 -1.75 170.5 -0.26 9 237 234.3 -1.14 234.9 -0.89 10 235 234.5 -0.20 235.7 0.31 11 302 302.9 0.31 302.2 0.08 12 162 167.5 3.37 166.2 2.59 13 166 166.8 0.46 163.1 -1.73 14 235 234.1 -0.40 235.5 0.22 15 309 303.2 -1.86 305.3 -1.19 16 307 303.5 -1.15 306.6 -0.12 17 164 166.2 1.36 166.2 1.36 18 231 233.5 1.10 231.6 0.26
27 ASME Boiler and pressure vessel code: section II- part D
properties (ASME, New York), (2015).
28 ASTM E 21–09: Standard test methods for elevated
temperature tension tests of metallic materials (ASTM
International, New York), (2009).
29 Javadi Y, Smith M C, Abburi Vnkata K, Naveed N, Forsey A N & Francis J A, et al., Int J Pres Ves Pip, 154 (2017) 41. 30 Rossini N S, Dassisti M, Benyounis K & Olabi A G,
Mater Des, 35 (2011) 572.
31 Malik A, Qureshi E, Dar N & Khan I, Thin Wall Struct, 46 (2008) 1391.
32 Goldak J & Akhlaghi M, Computational welding mechanics, Springer (2005), ISBN: 978-0-387-23288-1.
33 DuPont J N & Marder A R, Weld J, 74 (1995) 406s.
34 Roy R K, Design of experiments using the taguchi approach:
16 steps to product and process improvement , John Wiley &
Sons (2001), ISBN: 978-0-471-36101-5.
35 Ghani JA, Jamaluddin H, Rahman M N & Deros B,
Asian J Sci Res, 6 (2013) 27.
36 Meseguer-Valdenebro J, Portoles A & Oñoro J, Indian J Eng